SCIENTIFIC REPpRTS

open Tuning the Electronic Structure of Anatase Through Fluorination

Dario CorradinT, Damien Dambournet & Mathieu Salanne

A highly fluorinated anatase lattice has been recently reported, providing a new class of materials whose general chemical formula is Ti1_x^xX4XO2_4X (X- = F- or OH-). To characterise the complex structural features of the material and the different F environments, we here apply a computational screening procedure. After deriving a polarisable force—field from DFT simulations, we screen in a step-wise fashion a large number of possible configurations differing in the positioning of the titanium vacancies (□) and of the fluorine atoms. At each step only 10% of the configurations are retained. At the end of the screening procedure, a configuration is selected and simulated using DFT-based molecular dynamics. This allows us to analyse the atomic structure of the material, which is strongly disordered, leading to a strong decrease (by 0.8 eV) of the band gap compared to conventional anatase.

Titanium dioxide, TiO2, is a widely studied material. TiO2 has in fact several promising applications, for example in the fields of photocatalysis, green chemistry and energy storage1-8. Naturally occurring polymorphs of TiO2 include rutile, anatase and brookite. Recently, interest in the polymorphs of TiO2 has been sparked in particular by their possible application as anodic materials in Li ion batteries9-14. Fluorinated TiO2 has also been investigated15-20 since the presence of F in the compound might improve the sought characteristics of the material17 or stabilise the highly reactive {001} facets of the anatase crystal19,21. The nature of the fluorinated compound depends strongly on the fluorination technique employed18,22. So far, the stabilisation of fluorine within the anatase lattice of TiO2 has been poorly understood, probably because of the structural complexity of the fluorinated material.

Pure anatase is a tetragonal crystal, with c — 2.5a, and its lattice is characterised by TiO6 octahedral units. Recently, a novel synthesis technique conducted in our laboratory23 has led to the preparation of a highly fluorinated anatase material in which fluoride or hydroxide anions replace the oxides in their lattice sites and the resulting charge deficiency is compensated by the formation of a cationic vacancy (□) every four substitutions. The material obtained has thus the general formula Ti1-J^xX4xO2-4x, where X- = F- or OH- (the amount of F- may vary depending on the synthesis conditions). Elemental analysis and synchrotron diffraction have revealed the existence of more than 20% cation vacancies. In fact the stoichiometric formula Ti078^a22Xa88OL12 has been assigned to the most fluorinated composition of the material. By using 19F NMR spectroscopy, it has also been possible to discern three different coordination modes for the F atoms: F - Ti1^2, F - Ti2^1 and F - Ti3, highlighting the complex structural arrangement present in the material.

Here we report the results of a computational study of the fully-fluorinated, hydroxide-free material (i.e. Tia78Q,.22F0.88OL12) performed in order to better characterise its structural features and the effect of fluorination on the electronic structure. The enormous number of possible structural arrangements of the vacancies and of the F atoms in the anatase structure render the problem untreatable directly by ab initio simulations. Therefore we apply a screening procedure on the possible configurations of the material, in the spirit of the emerging high—throughput techniques24-26, by using classical Molecular Dynamics (MD). Several force—fields have been previously proposed for pure TiO227-33. In this work, we

Sorbonne Universités, UPMC Univ Paris 06, CNRS, UMR 8234, PHENIX, Paris, France. Current address: Laboratoire PASTEUR, UMR 8640 ENS-CNRS-UPMC Paris 6, Département de Chimie, École Normale Supérieure, 75005 Paris, France. Correspondence and requests for materials should be addressed to D.C. (email: dario.corradini@ens.fr) or M.S. (email: mathieu.salanne@upmc.fr)

Received: 02 March 2015 Accepted: 20 May 2015 Published: 26 June 2015

use a polarisable force—field valid for the pure phase34 as well as for the fluorinated material. We have extracted its parameters from Density Functional Theory (DFT) simulations, via a well-established force and dipole fitting procedure35,36. We have chosen to derive a new force—field instead of using an already available one for TiO2. This is motivated by the fact that we want the force—field to be compatible with O to F substitutions, as well as with other oxide species, e.g. SiO2, for future studies34. The details on the force—field employed are discussed in Supplementary Section S1, while an additional validation of the parameters involving fluorine atoms is presented in Supplementary Section S2.

In order to generate fluorinated samples starting from the pure TiO2 anatase, we apply a screening procedure, similar in spirit to what done by Wilmer et al. for metal-organic frameworks37 or by Coudert for zeolites38. At the fixed target composition Tia78E0.22F0.88OL12, we consider samples containing F in all possible environments F — Ti1D2, F — Ti2D1, and F — Ti3, as suggested by NMR23. We leave the ratio of F in the different environments free to vary at random. The starting fluorinated structures are generated from the 4 x 4 x 2 pure anatase TiO2 structure39 (Ti128O256) leading to a system thus composed: Ti100^28F112O144. We generate these configurations by erasing 28 Ti ions at random with no constraints on the creation of adjacent vacancies and we randomly substitute 112 O with 112 F. We impose that all F and O must be attached to at least one Ti.

The screening procedure is then initiated. The protocol is as follows:

(1) we perform single-point energy calculations on —1.5 • 105 configurations; we then retain the — 1.5 • 104 configurations with the lowest energy for the following step.

(2) we perform 0 K geometry optimisations of the atomic positions, keeping the length of the cell vectors fixed; we retain at maximum the 1.5 • 103 configurations with the lowest energy for the following step.

(3) we perform 0 K cell optimisations of both the atomic positions and the lengths of the cell vectors, while keeping the box angles fixed at a = 3 = y = n/2; we retain at maximum the 1.5 • 102 configurations with the lowest energy for the following step.

(4) we temper the configurations performing 10 ps NVT runs at finite temperatures from Tl = 25 K to T12 = 300 K, every AT = 25 K. The 15 configurations with the lowest energy at T12 = 300 K are retained for the following step.

(5) for the remaining samples, we perform a series of longer MD simulations at 300 K, first in the NVT and then in the NPT ensemble.

(6) we then simulate the configuration with the lowest potential energy for 10 ps using using DFT—based molecular dynamics. We extract structural (bond length, fluorine environments) and electronic (density of states) characteristics of the material from this simulation.

Testing all the starting configurations in a generic, entirely ab initio based high-throughput procedure would be impossible. Generally, such studies involve static calculations only since performing ab initio MD simulations is computationally too expensive. Nevertheless, it is interesting to test whether our selected configurations, i.e., the 10 configurations remaining at the end of step 5) of the screening procedure would have also been selected if ab initio static calculations had been performed. To test this, we take their initial structures and perform a full DFT relaxation. Then we take the same number of random configurations from the starting pool of configurations. We find that the configurations given by the classical screening all have a lower final DFT energy than the ones taken at random. The results of this validation are shown in Supplementary Fig. S2.

Next, we analyse how the initial structural arrangements correlate with the energy of the configurations. The results are shown in Fig. 1. We see that the lowest energies (at 0 K) correlate with a higher fraction of F — Ti2Dj. This is consistent with previous static DFT calculations performed on a system with only one vacancy and four O/F substitutions23, which showed that having the F closest to the vacancy stabilises the structure. In Fig. 1 we also report the initial energies of the best configurations given at the end by the screening procedure. We observe that these final screening configurations are found closer to the average F speciation values rather than at the highest F — Ti2Dj relative compositions. Some of them have strongly been stabilised during the procedure, showing the importance of taking into account relaxation and thermal effects (see also Supplementary Fig. S3).

In order to compare the structural properties of the material as found in the experiments with our simulations, we plot together the experimental x-ray structure factor S(k) and the one that we calculate from our trajectories using the Ashcroft—Langreth partial structure factors according to the formula:

where a,3 = Ti, O, F. xa are the relative atomic concentrations of atoms of type a, Sap(k) are the partial structure factors calculated from the simulation trajectories using

S tot (k)

SaP-JxOXpf a (k)f 3 (k) Sa33 (k) Sa xafa (k)

Sa3 (k) = (Pa (k) P3

Figure 1. Energy—structure relation. Fraction of F — Ti2^1 vs. energy of the configuration for the initial configurations at 0 K. The points are represented as small brown circles. For each different value of the fraction of F — Ti2^1 we calculate the mean (black circles) and the standard deviation (black bars) of the corresponding energies. We also report the values assumed at this stage by the configurations run at the final screening step (red squares).

Figure 2. Structure Factor. Comparison of the structure factor S(k) at ambient conditions measured in experiments (red line) and calculated from a DFT-based molecular dynamics simulation performed on the configuration selected by the screening procedure (black line).

where the dynamic variable p a (k) represents the Fourier component of the atomic density of type a atoms at wave vector k:

pa (k) = N-1 /2E exp (ik • r)

i=1 (3)

with r; the position of atom i, and Na the number of atoms of type a in the system. The angular brackets denote a thermal average, which was in practice evaluated as the time average over the whole simulation. Finally, fa(k) are the k-dependent atomic x—ray scattering factors. They are calculated using the analytic approximation:

Figure 3. Fluorine coordination number. Evolution of the proportion of each coordination mode for the fluorine during the DFT—based MD simulation. The cutoff distance for defining Ti—F neighbour atoms is set to 2.7 À.

-7 -6 -5-4-3-2-10 1 Energy (eV)

k Ti0 78D0 22^1.12^0.88

z^Total DOS

_7 -6 -5 -4 -3 -2 -1 0 1 2 3 4 5 Energy (eV)

Figure 4. Electronic density of states. Comparison of the total and ion-decomposed density of states of TiO2 (a) and Ti0.78D0.22OU2F0.88 (b) calculated using the HSE06 functional. Only the main contributions from the decomposition are shown. The plot for Ti0.78G0.22OU2F0.88 corresponds to the final snapshot of the simulation, shown on the right side. No significant changes have been observed for other snapshots, see Supplementary Fig. S5.

f a (k) = Ca + Eaa,/ eXP

; and ca are taken from Ref. 40 for O2 and from Ref. 41 for Ti4+ and F . The structure factor calculated from the DFT-based molecular dynamics simulation performed on the

where the coefficients aa/, ba

•—\ *H w"

S ^ (Dû 3

r (À) r (À)

Figure 5. Radial distribution functions. Partial radial distribution functions gap(r) at ambient conditions calculated from a classical MD simulation of pure TiO2 anatase (black) and from a DFT-based simulation of the configuration selected by the screening procedure (red).

final configuration is compared to the experimental signal in Fig. 2. The agreement between the two sets of data is good, taking into account that the experiments have been performed on nanoparticles, which leads to a strong broadening of the peaks, and that part of the fluoride ions are replaced by hydroxide groups. This may also affect the comparison, notwithstanding that F and OH are isoelectronic and thus their contribution to x-ray diffraction should not differ much if they occupy similar sites.

We also calculate the speciation of fluoride during the DFT-based molecular dynamics simulation. Contrarily to the initial configurations analysed in Fig. 1, the local relaxation of the F atoms (especially around the vacancies) leads to a wide distribution of Ti—F distances. It is therefore necessary to introduce a cutoff distance for assigning an environment to the F atoms. In Fig. 3 we show the time evolutions of the concentrations of F — Ti^2, F — Ti2^1 and F — Ti3 for a cutoff of 2.7 A which corresponds to the first minimum of the Ti—F radial distribution function. We observe that after 2 ps of simulation, the concentrations equilibrate around average values of 13/66/21% for F — Ti1^2, F — Ti2^1 and F — Ti3 respectively. This compares very well with the percentages measured by NMR in the experimental sample, i.e., 13/70/17%23. We can therefore conclude that the structure yielded by our screening procedure is realistic. This allows us to analyse it further in order to predict the material properties. We note that the F — Ti^Hj average concentration is larger than the corresponding fraction in the initial pool of configurations as shown in Fig. 1, because the fluorine atoms positions relax around the titanium vacancies during the first 2 ps of the simulation. However, no strong lattice rearrangements are observed, as can be seen from Supplementary Fig. S4.

The electronic structure is of particular interest for many applications, since TiO2-based materials are widely used in photocatalysis. We have therefore calculated the electronic density of states of fluorinated anatase on a series of snapshots extracted from our DFT-based molecular dynamics simulation, and compared it with the case of pure TiO2 anatase. We have used the hybrid functional HSE0 642,43 for these calculations. In agreement with previous works44, we see in Fig. 4 that the valence band edge of pure TiO2 anatase is dominated by O 2p, and the conduction band edge is formed by Ti 3d. The band gap is much narrower in Ti078^a22OU2Fa88, by 0.8 eV. Unlike the case of conventional doping with heteroatoms45,

the additional 2p states associated with fluoride ions do not locate at the top of the valence band, but rather at its bottom. The strong narrowing of the band gap is therefore due to the different structure of the material. In a previous study on TiO2 nanocrystals, Chen et al. have shown that, due to the presence of structural disorder, their materials exhibit a band gap substantially smaller than the one of pure bulk materials46. It is very likely that similar effects are at play here.

The structural disorder is apparently at the origin of these strong electronic structure changes. To test this idea, in Fig. 5 we show the partial radial distribution functions at ambient conditions gap(r) for the simulated pure anatase TiO2 and for the fluorinated anatase configuration selected by the screening procedure. The effect of the disorder introduced by the vacancies is immediately evident looking at the gTi-Ti(r) and at the gO-O(r). The gTi-O(r) structure seems to be conserved to a large extent at least for the first two shells, although the presence of vacancies induces a shortening of the first neighbour distance. The effect of disorder is also clear when looking for example at the region in between the first two peaks. We also observe that on the one hand, gTi-O(r) and gTi-F(r) are very similar, and so are the gO-O(r), gF-F(r) and gO-F(r). This confirms that the fluorine atoms substitute the oxygen ones inside the anatase structure.

In conclusion, in order to characterise fluorinated anatase Ti0.78D0.22F0.88OL12, we have developed a screening procedure employing a polarisable force—field. It has allowed us (i) to select the best configurations starting from a very large pool (hundreds of thousands) of possible configurations; (ii) to reproduce the experimental structure, (iii) to study details of the partial atomic and electronic structure using DFT-based molecular dynamics. Our results show that fluorinated anatase has a highly disordered structure, which results in a lower band gap, by 0.8 eV, compared to conventional anatase. Therefore we conclude that fluorination appears as a very promising route for tuning material properties. This may be exploited for several applications, for example photocatalysis.

Methods

We have performed the classical simulations using the software CP2K (single point calculations/geometry/cell optimisations, i.e., steps 1) to 3) of the screening procedure) and the in-house simulation software PIMAIM (molecular dynamics simulations, step 4) and 5) of the screening procedure). We have cut off the short—range interactions at half the norm of the shortest box vector (or less in NPT runs). The time step for the integration of the equations of motion has been set to 1 fs.

The DFT-based MD simulation has also been performed using the software CP2K47, using the Quickstep algorithm. We have used the GGA PBE48 exchange-correlation functional and we have employed the DZVP-MOLOPT-SR-GTH basis set49. Moreover, we have used the Goedecker-Teter-Hutter50 pseudo-potentials; for Ti atoms, the electronic orbitals explicitly represented are 3s23p63d24s2, for O atoms 2s22p4 and for F atoms 2s22p5. We have set a plane wave cut-off of 400 Ry. We have added dispersive interactions through the use of the DFT-D3 correction51, with a cutoff radius of 30 A. We have accumulated the trajectory for 10 ps, with the simulations time step being 0.5 fs. We have conducted the simulation in the NVT ensemble with a target temperature of 300 K. We have calculated the electronic density of states on a series of snapshot extracted from the trajectory, using the HSE06 functional42,43.

References

1. Chen, X. & Mao, S. S. Titanium Dioxide Nanomaterials: Synthesis, Properties, Modification and Applications. Chem. Rev. 107, 2891-2959 (2007).

2. Kavan, L., Grätzel, M., Gilbert, S. E., Klemenz, C. & Scheel, H. J. Electrochemical and Photoelectrochemical Investigation of Single—Crystal anatase. J. Am. Chem. Soc. 118, 6716-6723 (1996).

3. O'Regan, B. & Grätzel, M. A Low—Cost, High—Efficiency Solar Cell Based on Dye-Sensitized Colloidal TiO2 Films. Nature 353, 737-740 (1991).

4. Fujishima, A. & Honda, K. Electrochemical Photolysis of Water at a Semiconductor Electrode. Nature 238, 37-38 (1972).

5. Hoffmann, M. R., Martin, S. T., Choi, W. & Bahnemann, D. W. Environmental Applications of Semiconductor Photocatalysis. Chem. Rev. 95, 69-96 (1995).

6. Kudo, A. & Miseki, Y. Heterogeneous Photocatalyst Materials for Water Splitting. Chem. Soc. Rev. 38, 253-278 (2008).

7. Ravelli, D., Dondi, D.,Fagnoni, M. & Albini, A. Photocatalysis. A Multi—Faceted Concept for Green Chemistry. Chem. Soc. Rev. 38, 1999-2011 (2009).

8. Kamat, P. V. TiO2 Nanostructures: Recent Physical Chemistry Advances. J. Phys. Chem. C 116, 11849-11851 (2012).

9. Wagemaker, M., Borghols, W. J. H. & Mulder, F. M. Large Impact of Particle Size on Insertion Reactions. A Case for Anatase LixTiO2. J. Am. Chem. Soc. 129, 4323-4327 (2007).

10. Yang, M.-C., Lee, Y.-Y., Xu, B., Powers, K. & Meng, Y. S. TiO2 Flakes as Anode Materials for Li—Ion—Batteries. J. Power Sources 207, 166-172 (2012).

11. Morgan, B. J. & Watson, G. W. Role of Lithium Ordering in the Li^TiO2 Anatase ^ Titanate Phase Transition. J. Phys. Chem. Lett. 2, 1657-1661 (2011).

12. Yildirim, H., Greeley, J. P. & Sankaranarayanan, S. K. R. S. Concentration—Dependent Ordering of Lithiated Amorphous TiO2. J. Phys. Chem. C 117, 3834-3845 (2013).

13. Morgan, B. J. & Madden, P. A. Lithium Intercalation into TiO2(B): A Comparison of LDA, GGA, and GGA+U Density Functional Calculations. Phys. Rev. B 86, 035147/1-035147/13 (2012).

14. Morgan, B. J. & Watson, G. W. GGA+U Description of Lithium Intercalation into Anatase TiO2. Phys. Rev. B 82, 144119/1144119/11 (2010).

15. Tosoni, S., Lamiel-Garcia, O., Hevia, D. F. & Illas, F. Theoretical Study of Atomic Fluorine Diffusion through Bulk TiO2 Polymorphs. J. Phys. Chem. C 117, 5855-5860 (2013).

16. Tosoni, S., Lamiel-Garcia, O., Hevia, D. F., Miguel, J. & Illas, F. Electronic Structure of F-doped Bulk Rutile, Anatase, and Brookite Polymorphs of TiO2. J. Phys. Chem. C 116, 12738-12746 (2012).

17. Samadpour, M. et al. Fluorine Treatment of TiO2 for Enhancing Quantum Dot Sensitized Solar Cell Performance. J. Phys. Chem. C 115, 14400-14407 (2011).

18. Czoska, A. M. et al. The Nature of Defects in Fluorine—Doped TiO2. J. Phys. Chem. C 112, 8951-8956 (2008).

19. Wang, Y. et al. A Selective Etching Phenomenon on {001} Faceted Anatase Titanium Dioxide Single Crystal Surfaces by Hydrofluoric Acid. Chem. Commun. 47, 2829-2831 (2001).

20. Wang, Y. et al. Nature of Visible—Light Responsive Fluorinated Titanium Dioxides. J. Mater. Chem. A 1, 12948-12953 (2013).

21. Yang, H. G. et al. Anatase TiO2 Single Crystals with a Large Percentage of Reactive Facets. Nature 453, 638-641 (2008).

22. Yang, S. & Halliburton, L. E. Fluorine Donors and Ti3+ Ions in TiO2 Crystals. Phys. Rev. B 81, 035204/1-035204/7 (2010).

23. Li, W. et al. High Substitution Rate in TiO2 Anatase Nanoparticles with Cationic Vacancies for Fast Lithium Storage. Under review (2015).

24. Curtarolo, S. et al. The High—Throughput Highway to Computational Materials Design. Nat. Mater. 12, 191-201 (2013).

25. Zakutayev, A. et al. Theoretical Prediction and Experimental Realization of New Stable Inorganic Materials Using the Inverse Design Approach. J. Am. Chem. Soc. 135, 10048-10054 (2013).

26. Rondinelli, J. M. et al. Accelerating Functional Materials Discovery. Am. Ceram. Soc. Bull. 92, 14-21 (2013).

27. Catlow, C. R. A., Freeman, C. M. & Royle, R. L. Recent Studies Using Static Simulation Techniques. Physica B 131, 1-12 (1985).

28. Catlow, C. R. A. & James, R. Disorder in TiO2_^. Proc. R. Soc. Lond. A 384, 157-173 (1982).

29. Mostoller, M. & Wang, J. C. Ionic Potential Models in Insulators Having the Rutile Structure. Phys. Rev. B 32, 6773-6786 (1985).

30. Matsui, M. & Akaogi, M. Molecular Dynamics Simulation of the Structural and Physical Properties of the Four Polymorphs of TiO2. Mol. Simulat. 6, 239-244 (1991).

31. Sawatari, H., Iguchi, E. & Tilley, R. Formation Energies of Point Defects in Rutile TiO2. J. Phys. Chem. Solids 43, 1147-1155 (1982).

32. Post, J. E. & Burnham, C. W. Ionic Modeling of Mineral Structures and Energies in the Electron Gas Approximation: TiO2 Polymorphs, Quartz Forsterite, Diopside. Amer. Miner. 71, 142-150 (1986).

33. Han, X. J. et al. Polarizable Interatomic Force Field for TiO2 Parametrized Using Density Functional Theory. Phys. Rev. B 81, 134108/1-134108/9 (2010).

34. Corradini, D., Ishii, Y., Ohtori, N. & Salanne, M. DFT—based polarizable force field for TiO2 and SiO2. Model. Simul. Mater. Sci. Eng. xx, xxxx-xxxx (2015).

35. Salanne, M. et al. Including Many-Body Effects in Models for Ionic Liquids. Theor. Chem. Acc. 131, 1143/1-1143/16 (2012).

36. Tazi, S. et al. A Transferable Ab Initio Based Force Field for Aqueous Ions. J. Chem. Phys. 136, 114507/1-114507/12 (2012).

37. Wilmer, C. E. et al. Large—Scale Screening of Hypothetical Metal—Organic Frameworks. Nat. Chem. 4, 83-89 (2012).

38. Coudert, F.-X. Systematic Investigation of the Mechanical Properties of Pure Silica Zeolites: Stiffness, Anisotropy, and Negative Linear Compressibility. Phys. Chem. Chem. Phys. 15, 16012-16018 (2013).

39. Horn, M., Schwerdtfeger, C. F. & Meagher, E. P. Refinement of the Structure of Anatase at Several Temperatures. Z. Kristallogr. 136, 273-281 (1972).

40. Hemmati, M., Wilson, M. & Madden, P. A. Structure of Liquid Al2O3 from a Computer Simulation Model. J. Phys. Chem. B 103, 4023-4028 (1999).

41. Wilson, A. J. C. editor, International Tables for X-Ray Crystallography (Kluwer Academic Publisher, Dordrecht, 1992).

42. Heyd, J., Scuseria, G. E & Ernzerhof, M. Hybrid Functionals Based on a Screened Coulomb Potential. J. Chem. Phys. 118, 8207-8215 (2003).

43. Heyd, J., Scuseria, G. E. & Ernzerhof, M. Erratum: "Hybrid Functionals Based on a Screened Coulomb Potential" [J. Chem. Phys. 118, 8207 (2003)]. J. Chem. Phys. 124, 219906 (2006).

44. Scanlon, D. O. et al. Band Alignment of Rutile and Anatase TiO2. Nat. Mater. 12, 798-801 (2013).

45. Harb, M., Sautet, P. & Raybaud, P. Origin of the Enhanced Visible-Light Absorption in N-Doped Bulk Anatase TiO2 from First-Principles Calculations. J. Phys. Chem. C 115, 19394-19404 (2011).

46. Chen, X., Liu, L., Yu, P. Y. & Mao, S. S. Increasing Solar Absorption for Photocatalysis with Black Hydrogenated Titanium Dioxide Nanocrystals. Science 331, 746-750 (2011).

47. VandeVondele, J. et al. QUICKSTEP: Fast and accurate density functional calculations using a mixed Gaussian and plane waves. Comp. Phys. Commun. 167, 103-128 (2005).

48. Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865-3868 (1996).

49. VandeVondele, J. & Hutter, J. Gaussian basis sets for accurate calculations on molecular systems in gas and condensed phases. J. Chem. Phys. 127, 114105/1-114105/9 (2007).

50. Goedecker, S., Teter, M. & Hutter, J. Separable dual-space Gaussian pseudopotentials. Phys. Rev. B 54, 1703-1710 (1996).

51. Grimme, S., Antony, J., Ehrlich, S. & Krieg, H. A consistent and Accurate Ab Initio Parametrization of Density Functional Dispersion Correction (DFT-D) for the 94 Elements H-Pu. J. Chem. Phys. 132, 154104/1-154104/19 (2010).

Acknowledgements

We thank François-Xavier Coudert for introducing us to the screening techniques. We thank Paul A. Madden, Benjamin J. Morgan and Benjamin Rotenberg for discussions. The research leading to these results has received funding from the the European Union through the FP7—framework (FLUOSYNES, Contract PCI-GA-2012-321879). We also thank Karena W. Chapman for providing the experimental S(k) data. The work done at the Advanced Photon Source, an Office of Science User Facility operated for the U.S. Department of Energy (DOE) Office of Science by Argonne National Laboratory, was supported by the U.S. DOE under Contract No. DE-AC02-06CH11357.

Author Contributions

D.C. and M.S. have designed research. D.C. has implemented the screening procedure and has performed most of the simulations. M.S. has conducted the band gap calculations. D.C. and M.S. have written the manuscript and prepared the figures. D.D. has provided the experimental input. All the authors have participated in the discussions and reviewed the manuscript.

Additional Information

Supplementary information accompanies this paper at http://www.nature.com/srep Competing financial interests: The authors declare no competing financial interests.

How to cite this article: Corradini, D. et al. Tuning the Electronic Structure of Anatase Through Fluorination. Sci. Rep. 5, 11553; doi: 10.1038/srep11553 (2015).

(J) | This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article's Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/